Torsion Testing. Objectives


 Amanda Hamilton
 1 years ago
 Views:
Transcription
1 Laboratory 4 Torsion Testing Objectives Students are required to understand the principles of torsion testing, practice their testing skills and interpreting the experimental results of the provided materials when failed under torsion. To determine the maximum shearing stress, shear stress at proportional limit, shear modulus or modulus of rigidity and relationships between torque and degree of rotation of the tested materials. Students are able to differentiate the ability of materials such as cast iron and brass to withstand torque prior to torsion failure. Analysis and interpretation of the test parameters obtained should be carried out in relation to the failure nature of each material. Students are capable of selecting materials for engineering applications associated with torsion. Mechanical metallurgy laboratory
2 1. Literature review In many areas of engineering applications, materials are sometimes subjected to torsion in services, for example, drive shafts, axles and twisted drills. Moreover, structural applications such as bridges, springs, car bodies, airplane fuselages and boat hulls are randomly subjected to torsion. The materials used in this case should require not only adequate strength but also be able to withstand torque in operation. Even though torsion test is not as universal as tension test and do not have any standardized testing procedure, the significance lies on particular engineering applications and for the study of plastic flow in materials. Torsion test is applicable for testing brittle materials such as tool steels and the test has also been used to determine the forgeability of the materials by means of torsion testing at elevated temperatures. 1.1 Torsion test Figure 1: Torsion in cylindrical bar [1]. Generally, torsion occurs when the twisting moment or torque is applied to a member according to figure 1. The torque is the product of tangential force multiplied by the radial distance from the twisting axis and the tangent, measured in a unit of N.m. In torsion testing, the relationship between torque and degree of rotation is graphically presented and parameters such as ultimate torsional shearing strength (modulus of rupture), shear strength at proportional limit and shear modulus (modulus of rigidity) are generally investigated. Moreover, fracture surfaces of specimens tested under torsion can be used to determine the characteristics of the materials whether it would fail in a brittle or a ductile manner. Mechanical metallurgy laboratory
3 Figure 2: Torsion testing machine [2]. In order to study the response of materials under a torsional force, the torsion test is performed by mounting the specimen onto a torsion testing machine as shown in figures 24, and then applying the twisting moment till failure. The torque and degree of rotation are measured and plotted as shown in figure 5. It can be seen that higher torsional force is required at the higher degrees of rotation. Normally, the test specimens used are of a cylindrical rod type since the stress distribution across the section of the rod is the simplest geometry, which is easy for the calculation of the stresses. Both ends of the cylindrical specimen are tightened to hexagonal sockets in which one is fitted to a torque shaft and another is fitted to an input shaft. The twisting moment is applied by turning the input handwheel as illustrated in figure 3 to produce torque until the specimen fails. Mechanical metallurgy laboratory
4 Figure 3: Schematic diagram showing details of torsion testing machine [2] Figure 4: Torsion specimen [2] When the twisting moment is applied, the torque is reacted by a torque shaft, which moves in relation to the deflection arm. The movement of the deflection arm is measured by a linear potentiometer, which is connected to a calibrated TQ digital torque meter to give a readout of the torque in a unit of Nm or lb.in. The more we turn the input handwheel clockwise to increase the degree of rotation, the more torque is produced. At the initial stage, the graphical relationship of the torque and degree of rotation measured is linear as demonstrated in figure 5. The specimen is Mechanical metallurgy laboratory
5 elastically deformed and the recovery of the specimen to its original shape is possible if the specimen is unloaded. However, if a high degree of rotation is applied passing a proportional limit, the specimen starts to deform plastically and will not return to its original shape when the input handwheel is turned anticlockwise. The degree of rotation can be read out from two protractors, elastic and plastic range protractors. First, an elastic range protractor scale is fitted on the input handwheel connected to the input shaft of the gear box. This protractor scale provides an accurate reading of 0.1 o and thus one revolution represents 6 o. A resettable revolution counter is fitted to the gearbox to record the overall input revolutions. When the twisting moment is large, the second protractor scale is required for the readouts in the plastic range of deformation. The second protractor is fitted onto the output shaft and provides a reading of 1 o with one revolution representing 360 o. Figure 5: Relationship between torque and angle of twist [2]. Considering a cylindrical bar with one end being twisted as shown in figure 6, the twisting moment M T is resisted by the shear stress τ existing across the specimen section. This shear stress is zero at the center of the bar, increases linearly with its radius and finally reaches its maximum value at the peripheral of the bar. If the cylindrical bar with a length of L, the twisting moment can be related to the shear stress as follow Mechanical metallurgy laboratory
6 M T J Gθ τ = L r = (1) The shear strain, γ, can be calculated from equation 2 rθ γ =tan θ = (2) L where J is the polar moment of inertia, mm 2 or in 2 G is the shear modulus, N/mm 2 or lbf/in 2 θ r L is degree of rotation, radian is the radius of the cylindrical bar, mm or in is the length of the cylindrical bar, mm or in τ is the shear stress, N/mm 2 or lbf/in 2 Figure 6: Torsion of a solid bar [3]. According to the graphical relationship of torque and degree of rotation, we can notice that the torsion specimen deformed elastically and then plastically similar to the case of the tension tested specimen. The initial stage of elastic behavior shows a linear relationship of torque and degree of rotation with its slope representing the shear modulus of the modulus of rigidity, G. The stress at the proportional limit is frequently determined at 0.04 rad.m 1 of the gauge length. Beyond the proportional limit, specimen deformed in a plastic manner and the relationship between the torque and the degree of rotation is no longer linear. However the determination of the proportional limit carried out using a torsional specimen of a thinwall tube type will provides a more accurate value in comparison to that obtained from a cylindrical rod type specimen. Since the stresses vary across the section of the specimen from the center toward the peripheral of the specimen as mentioned Mechanical metallurgy laboratory
7 previously, the reduced effect of stress distribution in the thinwalled specimen is therefore beneficial for the calculation of the stress. Within the elastic range of deformation, the shear stress can be calculated according to equation 1 M T r = J τ (3) For a solid cylindrical specimen, the polar moment J = πd 4 /32, we can therefore determine the shear stress as shown in equation 4 MTD/ 2 16M τ = 4 πd / 32 πd = (4) T 3 For a tube specimen, the maximum shear stress at the peripheral of the tube can be calculated from equation 5 16M 1 = T π 4 ( D D D τ (5) ) where D 1 D 2 is the outer diameter of the tube is the inner diameter of the tube Therefore, if the torque and the degree of rotation are known according to the experimental result, the shear stress and the shear strain can be determined from equations 2 and 4. The obtained information is then used for the construction of the graphical relationship between the modular shear stress (16M T /ad 3 ) and the shear strain (θr/l) as illustrated in figure 7. The curve is somewhat similar to those typical stressstrain curves tested under tension, giving elastic and plastic ranges with respect to the torsional stress applied. Nevertheless, the calculated shear stress according to equation 4 is only suitable for the evaluation of the stresses in the elastic range. The plastic stress obtained from the shear stressshear strain curve is therefore larger than the real stress. Furthermore, in the case that there is a large amount of plastic deformation involved, the length of the specimen is considerably changed, which can result in the superposition of the longitudinal stresses on the torsional shear stresses. Even Mechanical metallurgy laboratory
8 though, the former is considered to be small and can be neglected, they might also affect the torsional failure strain of the specimen. Nadai [3] has proposed the method for the calculation of the stress in the plastic range from a known torquedegree of rotation curve as expressed in equation 6 3M τ = (6) u max 3 2πa where M max a is the maximum twisting moment is the distance from the center to the peripheral of the specimen according to figure 4. Figure 7: Relationship between modular shear stress and shear strain [2]. 1.2 Types of torsion failures Torsion failures are different from tension failures and normally provide little deformation or elongation. The characteristic of the fracture surface is related to the state of stress at the point on the bar surface, which can be described as shown in figure 8. It can be seen that the maximum shear stresses exist along two planes, which are perpendicular to each other. One is perpendicular to the longitudinal axis (yy) and another is aligned parallel to the longitudinal axis (xx). The principle Mechanical metallurgy laboratory
9 stresses σ 1 and σ 3 are inclined at 45 o to the longitudinal axis and have their magnitudes equal to those of the shear stresses. The principle stress σ 1 is tensile while the principle stress σ 3 is compressive. The intermediate stress σ 2 is zero under torsion. As mentioned previously, the characteristics of torsion fractures are influenced by torsional and tensile forces. These result in two types of torsion failures; 1) ductile failure due to the shear stresses and 2) brittle failure due to the tensile stresses. The former produces the fracture surface along the plane of the maximum shear stress and more frequently normal to the longitudinal axis as shown in figures a) and b). The latter exhibits the fracture planes normal to the directions of the tensile stresses, which are 45 o to the longitudinal axis. Figure 9 shows brittle and ductile fracture surfaces observed from a driveshaft and a brass rod respectively failed under torsion. This means the driveshaft failed under a brittle manner influenced by the tensile stresses while the ductile failure of the brass rod was affected by the shear stresses. However, if the specimen fails into little pieces where the fracture plane cannot be determined, the fracture in this case is considered to start along the maximum shear stress parallel to the longitudinal axis of the specimen. In addition, it has also been shown in a study, which has indicated that the fracture characteristic is associated with the hardness of the tool steels. If the tool steel possesses the hardness values of higher than 720 VHN, failure is expected to be influenced by tensile stress. Conversely, if the hardness of the tool steel is lower than 720 VHN, the shear stress is responsible for such a failure. Figure 8: Types of failure in torsion [3]. Mechanical metallurgy laboratory
10 Figure 9: Fracture surfaces of a driveshaft and a brassrod failed in brittle and ductile manners under torsion. 1.3 Calibration of the torsion test machine Prior to torsion testing, calibration of the testing machine should be carried out as follows Put the calibration arm onto the square end of the torque shaft and level it by adjusting the handwheel as demonstrated in figure 10. Zero the dial gauge Set the digital meter for torque measurement to SI unit and adjust the readout to zero by turning the knob at the rear of the device Add a 5 kg load to the calibration arm and adjust the dial gauge to zero by rotating the handwheel. The reading on the digital meter should be 24.5± 0.5 Nm. If the error is higher than 0.5 Nm, the CAL screw at the rear of the instrument should be adjusted to set the reading back to 24.5 Nm. (Note: the calibration arm = 500 mm, load = 5 kg, thus the torque = 5 x 9.81 x 0.5 = 24.5 Nm) Remove the load and check that the reading now returns to zero The full range calibration can be carried out by putting the available weights of 500 g, 1 kg and 2 kg incrementally while the reading of torque of each increment should be recorded. The obtained values should be within the tolerance of ± 0.5 Nm of the calculated values Plot the graph of the torque reading against the applied torque (0.5 x load x 9.81), giving a linear relationship. Calculate the slope which should be approximately unity. Mechanical metallurgy laboratory
11 Figure 10: Calibration of the torsion testing machine [2]. Mechanical metallurgy laboratory
12 2. Materials and equipment 2.1 Test specimens 2.2 Micrometer or vernia caliper 2.3 Permanent pen 2.4 Torsion testing machine 3. Experimental Procedure 3.1 Measure initial diameter, initial length and initial gauge length of the specimen. Record these parameters on the table provided. 3.2 Draw a line using a permanent pen along the length of the test specimen. This line will help to notice the degree of rotation during applying the twisting moment. 3.3 Calibrate the testing equipment following section Grip the test specimen on to the torsion testing machine using hexagonal sockets and make sure the specimens are firmly mounted. Fit both ends of the specimen to input and torque shafts and set reading on the torque meter to zero. 3.5 Start twisting the specimen at strain increment of 0.5 o until failure occurs. Record the received data rotation in the table provided for the construction of torque and degree relationship 3.6 Construct the relationship between shear stress and shear strain. Determine maximum shear stress, shear stress at proportional limit and modulus of rigidity. 3.7 Sketch fracture surfaces of failed specimens and described their natures in the table provided. 3.8 Discuss and conclude the obtained experimental results. Mechanical metallurgy laboratory
13 4. Results Details Cast iron Brass Initial diameter (mm) Final diameter (mm) Initial gauge length (mm) Final gauge length (mm) Initial overall length of specimen (mm) Final overall length of specimen (mm) Strain increment (degree) Maximum torque (Nm) Maximum shear stress (MPa) Shear stress at proportional limit (MPa) Modulus of rigidity (GPa) Fracture surface details Table 1 Experimental results for torsion test of cast iron and brass. Mechanical metallurgy laboratory
14 5. Discussion Mechanical metallurgy laboratory
15 6. Conclusions Mechanical metallurgy laboratory
16 7. Questions 7.1 Did cast iron and brass fail in different fracture manners? Explain. 7.2 What are the differences between torsion and tension tests? Mechanical metallurgy laboratory
17 7.3 Which engineering applications do you think that torsion test is vital? Give three examples. 8. References SM1/2 Torsion testing machine, TecQuipment Ltd Dieter, G.E., Mechanical metallurgy, 1988, SI metric edition, McGrawHill, ISBN Mechanical metallurgy laboratory
Torsion Tests. Subjects of interest
Chapter 10 Torsion Tests Subjects of interest Introduction/Objectives Mechanical properties in torsion Torsional stresses for large plastic strains Type of torsion failures Torsion test vs.tension test
More informationTensile Testing. Objectives
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationStress Strain Relationships
Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationPLASTIC DEFORMATION AND STRESSSTRAIN CURVES
PLASTIC DEFORMATION AND STRESSSTRAIN CURVES Introduction Background Unit: Plastic Deformation and StressStrain Curves In the last unit we studied the elastic response of materials to externally applied
More informationSolid Mechanics. Stress. What you ll learn: Motivation
Solid Mechanics Stress What you ll learn: What is stress? Why stress is important? What are normal and shear stresses? What is strain? Hooke s law (relationship between stress and strain) Stress strain
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationStress and Deformation Analysis. Representing Stresses on a Stress Element. Representing Stresses on a Stress Element con t
Stress and Deformation Analysis Material in this lecture was taken from chapter 3 of Representing Stresses on a Stress Element One main goals of stress analysis is to determine the point within a loadcarrying
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationMAE 20 Winter 2011 Assignment 5
MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the
More informationStructures and Stiffness
Structures and Stiffness ENGR 10 Introduction to Engineering Ken Youssefi/Thalia Anagnos Engineering 10, SJSU 1 Wind Turbine Structure The Goal The support structure should be optimized for weight and
More informationAdam Zaborski handouts for Afghans
Tensile test Adam Zaborski handouts for Afghans Outline Tensile test purpose Universal testing machines and test specimens Stressstrain diagram Mild steel : proportional stage, elastic limit, yielding
More informationPlastic Behaviour  Tensile Strength
Plastic Behaviour  Tensile Strength Transition of mechanical behaviour from elastic to plastic depends upon the material type and its condition as tested (hotrolled, coldrolled, heat treated, etc.).
More informationENGINEERING COUNCIL CERTIFICATE LEVEL
ENGINEERING COUNCIL CERTIICATE LEVEL ENGINEERING SCIENCE C103 TUTORIAL  BASIC STUDIES O STRESS AND STRAIN You should judge your progress by completing the self assessment exercises. These may be sent
More informationMECHANICAL PRINCIPLES HNC/D PRELIMINARY LEVEL TUTORIAL 1 BASIC STUDIES OF STRESS AND STRAIN
MECHANICAL PRINCIPLES HNC/D PRELIMINARY LEVEL TUTORIAL 1 BASIC STUDIES O STRESS AND STRAIN This tutorial is essential for anyone studying the group of tutorials on beams. Essential prerequisite knowledge
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationIntroduction, Method of Sections
Lecture #1 Introduction, Method of Sections Reading: 1:12 Mechanics of Materials is the study of the relationship between external, applied forces and internal effects (stress & deformation). An understanding
More informationCOMPLEX STRESS TUTORIAL 3 COMPLEX STRESS AND STRAIN
COMPLX STRSS TUTORIAL COMPLX STRSS AND STRAIN This tutorial is not part of the decel unit mechanical Principles but covers elements of the following sllabi. o Parts of the ngineering Council eam subject
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME 2 ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
More informationShaft Design. Shaft Design. Shaft Design Procedure. Chapter 12
Shaft Design Chapter 1 Material taken from Mott, 003, Machine Elements in Mechanical Design Shaft Design A shaft is the component of a mechanical device that transmits rotational motion and power. It is
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationDESIGN AND DEVELOPMENT OF AN ECONOMICAL TORSION TESTING MACHINE
DESIGN AND DEVELOPMENT OF AN ECONOMICAL TORSION TESTING MACHINE by GLENN E. VALLEE ASSISTANT PROFESSOR MECHANICAL ENGINEERING and ROBERT SHORT WESTERN NEW ENGLAND COLLEGE SPRINGFIELD MASSACHUSSETS Session
More informationENGINEERING COUNCIL CERTIFICATE LEVEL ENGINEERING SCIENCE C103 TUTORIAL 3  TORSION
ENGINEEING COUNCI CETIFICATE EVE ENGINEEING SCIENCE C10 TUTOIA  TOSION You should judge your progress by completing the self assessment exercises. These may be sent for marking or you may request copies
More informationChapter 12 Elasticity
If I have seen further than other men, it is because I stood on the shoulders of giants. Isaac Newton 12.1 The Atomic Nature of Elasticity Elasticity is that property of a body by which it experiences
More informationCH 6: Fatigue Failure Resulting from Variable Loading
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
More informationσ = F / A o Chapter Outline Introduction Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? and Tension Compression Shear Torsion Elastic deformation Chapter Outline Introduction To understand and describe how materials
More informationSAMPLE FORMAL LABORATORY REPORT. Fatigue Failure through Bending Experiment Adapted from a report submitted by Sarah Thomas
SAMPLE FORMAL LABORATORY REPORT Fatigue Failure through Bending Experiment Adapted from a report submitted by Sarah Thomas Lab Partners: David Henry and James Johnson ME 498 November 10, 2004 Professor
More informationMechanical Metallurgy
Mechanical Metallurgy Lecturer Assessment Dr. Assignment 20 (homework, quiz, attendance) Midterm exam 40 Final exam 40 Total 100 Mechanical Metallurgy Subject of interests Part I Mechanical fundamentals
More informationB.TECH. (AEROSPACE ENGINEERING) PROGRAMME (BTAE) TermEnd Examination December, 2011 BAS010 : MACHINE DESIGN
No. of Printed Pages : 7 BAS01.0 B.TECH. (AEROSPACE ENGINEERING) PROGRAMME (BTAE) CV CA CV C:) O TermEnd Examination December, 2011 BAS010 : MACHINE DESIGN Time : 3 hours Maximum Marks : 70 Note : (1)
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQF LEVEL 3 OUTCOME 1  LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS
EDEXCEL NATIONAL CERTIICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQ LEVEL 3 OUTCOME 1  LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS 1. Be able to determine the effects of loading in static engineering
More informationFatigue Failure Due to Variable Loading
Fatigue Failure Due to Variable Loading Daniel Hendrickson Department of Computer Science, Physics, and Engineering University of Michigan Flint Advisor: Olanrewaju Aluko 1. Abstract Fatigue failure in
More informationCourse 1 Laboratory. Second Semester. Experiment: Young s Modulus
Course 1 Laboratory Second Semester Experiment: Young s Modulus 1 Elasticity Measurements: Young Modulus Of Brass 1 Aims of the Experiment The aim of this experiment is to measure the elastic modulus with
More informationsuperimposing the stresses and strains cause by each load acting separately
COMBINED LOADS In many structures the members are required to resist more than one kind of loading (combined loading). These can often be analyzed by superimposing the stresses and strains cause by each
More informationMCE380: Measurements and Instrumentation Lab. Chapter 9: Force, Torque and Strain Measurements
MCE380: Measurements and Instrumentation Lab Chapter 9: Force, Torque and Strain Measurements Topics: Elastic Elements for Force Measurement Dynamometers and Brakes Resistance Strain Gages Holman, Ch.
More informationPOWER SCREWS (ACME THREAD) DESIGN
POWER SCREWS (ACME THREAD) DESIGN There are at least three types of power screw threads: the square thread, the Acme thread, and the buttress thread. Of these, the square and buttress threads are the most
More informationTorque and Rotary Motion
Torque and Rotary Motion Name Partner Introduction Motion in a circle is a straightforward extension of linear motion. According to the textbook, all you have to do is replace displacement, velocity,
More information15. MODULUS OF ELASTICITY
Chapter 5 Modulus of Elasticity 5. MODULUS OF ELASTICITY The modulus of elasticity (= Young s modulus) E is a material property, that describes its stiffness and is therefore one of the most important
More informationProperties of Materials
CHAPTER 1 Properties of Materials INTRODUCTION Materials are the driving force behind the technological revolutions and are the key ingredients for manufacturing. Materials are everywhere around us, and
More informationMechanical Properties
Mechanical Properties Hardness Hardness can be defined as resistance to deformation or indentation or resistance to scratch. Hardness Indentation Scratch Rebound Indentation hardness is of particular interest
More informationME 215 Engineering Materials I
ME 215 Engineering Materials I Chapter 3 Properties in Tension and Compression (Part III) Mechanical Engineering University of Gaziantep Dr. A. Tolga Bozdana www.gantep.edu.tr/~bozdana True Stress and
More informationHardness Testing. Objectives
Laboratory 2 Hardness Testing Objectives Students are required to understand the principles of hardness testing, i.e., Rockwell, Brinell and Vickers hardness tests. Students are able to explain variations
More informationTensile Testing Laboratory
Tensile Testing Laboratory By Stephan Favilla 0723668 ME 354 AC Date of Lab Report Submission: February 11 th 2010 Date of Lab Exercise: January 28 th 2010 1 Executive Summary Tensile tests are fundamental
More informationLab 7: Rotational Motion
Lab 7: Rotational Motion Equipment: DataStudio, rotary motion sensor mounted on 80 cm rod and heavy duty bench clamp (PASCO ME9472), string with loop at one end and small white bead at the other end (125
More informationYield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials. τ xy 2σ y. σ x 3. τ yz 2σ z 3. ) 2 + ( σ 3. σ 3
Yield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials Brittle materials are materials that display Hookean behavior (linear relationship between stress and strain) and which
More informationTHE COMPOSITE DISC  A NEW JOINT FOR HIGH POWER DRIVESHAFTS
THE COMPOSITE DISC  A NEW JOINT FOR HIGH POWER DRIVESHAFTS Dr Andrew Pollard Principal Engineer GKN Technology UK INTRODUCTION There is a wide choice of flexible couplings for power transmission applications,
More informationMATERIALS SELECTION FOR SPECIFIC USE
MATERIALS SELECTION FOR SPECIFIC USE1 Subtopics 1 Density What determines density and stiffness? Material properties chart Design problems LOADING 2 STRENGTH AND STIFFNESS Stress is applied to a material
More informationLab for Deflection and Moment of Inertia
Deflection and Moment of Inertia Subject Area(s) Associated Unit Lesson Title Physics Wind Effects on Model Building Lab for Deflection and Moment of Inertia Grade Level (1112) Part # 2 of 3 Lesson #
More informationLecture Slides. Chapter 8. Screws, Fasteners, and the Design of Nonpermanent Joints
Lecture Slides Chapter 8 Screws, Fasteners, and the Design of Nonpermanent Joints The McGrawHill Companies 2012 Chapter Outline Reasons for Nonpermanent Fasteners Field assembly Disassembly Maintenance
More informationCHAPTER 9 : MECHANICAL PROPERTIES OF SOLIDS ONE MARK QUESTIONS: 1. What is elasticity of a body? 2. What is plasticity? 3. Which property of a body
1 CHAPTER 9 : MECHANICAL PROPERTIES OF SOLIDS ONE MARK QUESTIONS: 1. What is elasticity of a body? 2. What is plasticity? 3. Which property of a body is responsible for regaining original shape and size
More informationForce measurement. Forces VECTORIAL ISSUES ACTION ET RÉACTION ISOSTATISM
Force measurement Forces VECTORIAL ISSUES In classical mechanics, a force is defined as "an action capable of modifying the quantity of movement of a material point". Therefore, a force has the attributes
More informationWelcome to the first lesson of third module which is on thinwalled pressure vessels part one which is on the application of stress and strain.
Strength of Materials Prof S. K. Bhattacharya Department of Civil Engineering Indian Institute of Technology, Kharagpur Lecture 15 Application of Stress by Strain Thinwalled Pressure Vessels  I Welcome
More informationMATERIALS AND MECHANICS OF BENDING
HAPTER Reinforced oncrete Design Fifth Edition MATERIALS AND MEHANIS OF BENDING A. J. lark School of Engineering Department of ivil and Environmental Engineering Part I oncrete Design and Analysis b FALL
More informationSTRESS AND DEFORMATION ANALYSIS OF LINEAR ELASTIC BARS IN TENSION
Chapter 11 STRESS AND DEFORMATION ANALYSIS OF LINEAR ELASTIC BARS IN TENSION Figure 11.1: In Chapter10, the equilibrium, kinematic and constitutive equations for a general threedimensional solid deformable
More informationMCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions
MCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions The Quiz questions based upon HW9 will open on Thursday, Apr. 11 and close on Wednesday, Apr 17 at 1:30 PM. References to A&J: Chapters 13,
More informationUnit 2: Science for Engineering LO4: Understand properties of materials  Forceextension graphs Instructions and answers for teachers
Unit 2: Science for Engineering LO4: Understand properties of materials  Forceextension graphs Instructions and answers for teachers These instructions should accompany the OCR resource Forceextension
More informationPhysics 41, Winter 1998 Lab 1  The Current Balance. Theory
Physics 41, Winter 1998 Lab 1  The Current Balance Theory Consider a point at a perpendicular distance d from a long straight wire carrying a current I as shown in figure 1. If the wire is very long compared
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationMECHANICS OF SOLIDS COMPRESSION MEMBERS TUTORIAL 1 STRUTS. On completion of this tutorial you should be able to do the following.
MECHANICS OF SOLIDS COMPRESSION MEMBERS TUTORIAL 1 STRUTS You should judge your progress by completing the self assessment exercises. On completion of this tutorial you should be able to do the following.
More informationEXPERIMENT: MOMENT OF INERTIA
OBJECTIVES EXPERIMENT: MOMENT OF INERTIA to familiarize yourself with the concept of moment of inertia, I, which plays the same role in the description of the rotation of a rigid body as mass plays in
More informationChapter 5: Tool Dynamometers
Chapter 5: Tool Dynamometers LEARNING OBJECTIVES Different types of transducers used in Dynamometers Design Requirements Types of Dynamometers 
More informationFatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY)
Fatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY) Ali Fatemi, Jonathan Williams and Farzin Montazersadgh Professor and Graduate
More informationP4 Stress and Strain Dr. A.B. Zavatsky MT07 Lecture 4 Stresses on Inclined Sections
4 Stress and Strain Dr. A.B. Zavatsky MT07 Lecture 4 Stresses on Inclined Sections Shear stress and shear strain. Equality of shear stresses on perpendicular planes. Hooke s law in shear. Normal and shear
More informationMUKAVEMET KIRILMA HİPOTEZLERİ
1 MUKAVEMET KIRILMA HİPOTEZLERİ 17. Theories of failure or yield criteria (1) Maximum shearing stress theory (2) Octahedral shearing stress theory (3) Maximum normal stress theory for brittle materials.
More informationConcepts of Stress and Strain
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original
More informationMENG 302L Lab 4: Modulus of Elasticity and Poisson s Ratio
MENG 302L Lab 4: Modulus of Elasticity and Poisson s Ratio Introduction: In Lab 4 we will measure the two fundamental elastic constants relating stress to strain: Modulus of Elasticity and Poisson s Ratio.
More informationBending Stress in Beams
93673600 Bending Stress in Beams Derive a relationship for bending stress in a beam: Basic Assumptions:. Deflections are very small with respect to the depth of the beam. Plane sections before bending
More informationStructural Axial, Shear and Bending Moments
Structural Axial, Shear and Bending Moments Positive Internal Forces Acting Recall from mechanics of materials that the internal forces P (generic axial), V (shear) and M (moment) represent resultants
More informationPROPERTIES OF MATERIALS
1 PROPERTIES OF MATERIALS 1.1 PROPERTIES OF MATERIALS Different materials possess different properties in varying degree and therefore behave in different ways under given conditions. These properties
More informationENGINEERING SCIENCE H1 OUTCOME 1  TUTORIAL 3 BENDING MOMENTS EDEXCEL HNC/D ENGINEERING SCIENCE LEVEL 4 H1 FORMERLY UNIT 21718P
ENGINEERING SCIENCE H1 OUTCOME 1  TUTORIAL 3 BENDING MOMENTS EDEXCEL HNC/D ENGINEERING SCIENCE LEVEL 4 H1 FORMERLY UNIT 21718P This material is duplicated in the Mechanical Principles module H2 and those
More informationMECHANICS OF SOLIDS  BEAMS TUTORIAL 2 SHEAR FORCE AND BENDING MOMENTS IN BEAMS
MECHANICS OF SOLIDS  BEAMS TUTORIAL 2 SHEAR FORCE AND BENDING MOMENTS IN BEAMS This is the second tutorial on bending of beams. You should judge your progress by completing the self assessment exercises.
More informationMechanical properties 3 Bend test and hardness test of materials
MME131: Lecture 15 Mechanical properties 3 Bend test and hardness test of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Bend test of brittle materials Hardness testing
More information, to obtain a way to calculate stress from the energy function U(r).
BIOEN 36 013 LECTURE : MOLECULAR BASIS OF ELASTICITY Estimating Young s Modulus from Bond Energies and Structures First we consider solids, which include mostly nonbiological materials, such as metals,
More informationChapter 10 Rotational Motion. Copyright 2009 Pearson Education, Inc.
Chapter 10 Rotational Motion Angular Quantities Units of Chapter 10 Vector Nature of Angular Quantities Constant Angular Acceleration Torque Rotational Dynamics; Torque and Rotational Inertia Solving Problems
More informationSHAFTS: TORSION LOADING AND DEFORMATION
ECURE hird Edition SHAFS: ORSION OADING AND DEFORMAION A. J. Clark Shool of Engineering Department of Civil and Environmental Engineering 6 Chapter 3.13.5 by Dr. Ibrahim A. Assakkaf SPRING 2003 ENES 220
More informationMIME 3330 Mechanics Laboratory LAB 5: ROTATING BENDING FATIGUE
MIME 3330 Mechanics Laboratory LAB 5: ROTATING BENDING FATIGUE Introduction In this experiment, the finite life fatigue behavior of a smooth cylindrical specimen as shown in Figure 1 will be studied in
More informationMECHANICS OF MATERIALS
T dition CHTR MCHNICS OF MTRIS Ferdinand. Beer. Russell Johnston, Jr. John T. DeWolf ecture Notes: J. Walt Oler Texas Tech University Stress and Strain xial oading  Contents Stress & Strain: xial oading
More informationCRITERIA FOR PRELOADED BOLTS
National Aeronautics and Space Administration Lyndon B. Johnson Space Center Houston, Texas 77058 REVISION A JULY 6, 1998 REPLACES BASELINE SPACE SHUTTLE CRITERIA FOR PRELOADED BOLTS CONTENTS 1.0 INTRODUCTION..............................................
More informationIntroduction to Mechanical Behavior of Biological Materials
Introduction to Mechanical Behavior of Biological Materials Ozkaya and Nordin Chapter 7, pages 127151 Chapter 8, pages 173194 Outline Modes of loading Internal forces and moments Stiffness of a structure
More informationMechanical Properties  Stresses & Strains
Mechanical Properties  Stresses & Strains Types of Deformation : Elasic Plastic Anelastic Elastic deformation is defined as instantaneous recoverable deformation Hooke's law : For tensile loading, σ =
More informationRotational Motion. Symbol Units Symbol Units Position x (m) θ (rad) (m/s) " = d# Source of Parameter Symbol Units Parameter Symbol Units
Introduction Rotational Motion There are many similarities between straightline motion (translation) in one dimension and angular motion (rotation) of a rigid object that is spinning around some rotation
More informationMechanics of Materials Summary
Mechanics of Materials Summary 1. Stresses and Strains 1.1 Normal Stress Let s consider a fixed rod. This rod has length L. Its crosssectional shape is constant and has area. Figure 1.1: rod with a normal
More informationSolution for Homework #1
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
More information8.2 Elastic Strain Energy
Section 8. 8. Elastic Strain Energy The strain energy stored in an elastic material upon deformation is calculated below for a number of different geometries and loading conditions. These expressions for
More informationDesign Analysis and Review of Stresses at a Point
Design Analysis and Review of Stresses at a Point Need for Design Analysis: To verify the design for safety of the structure and the users. To understand the results obtained in FEA, it is necessary to
More informationModule 5 Couplings. Version 2 ME, IIT Kharagpur
Module 5 Couplings Lesson 1 Introduction, types and uses Instructional Objectives At the end of this lesson, the students should have the knowledge of The function of couplings in machinery. Different
More informationREINFORCED CONCRETE. Reinforced Concrete Design. A Fundamental Approach  Fifth Edition
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition CONCRETE Fifth Edition A. J. Clark School of Engineering Department of Civil and Environmental Engineering
More informationSection 16: Neutral Axis and Parallel Axis Theorem 161
Section 16: Neutral Axis and Parallel Axis Theorem 161 Geometry of deformation We will consider the deformation of an ideal, isotropic prismatic beam the cross section is symmetric about yaxis All parts
More informationTSL Professional Services
Report For: Laboratory #: 40287605 5375 Edgeway Drive, ALLENDALE, MI, USA Report Date: December 21, 2005 49401 Received Date: November 3, 2005 Phone: 616 875 7725 Fax: 616 875 6009 Customer P.O. #: COD
More informationLinear Centripetal Tangential speed acceleration acceleration A) Rω Rω 2 Rα B) Rω Rα Rω 2 C) Rω 2 Rα Rω D) Rω Rω 2 Rω E) Rω 2 Rα Rω 2 Ans: A
1. Two points, A and B, are on a disk that rotates about an axis. Point A is closer to the axis than point B. Which of the following is not true? A) Point B has the greater speed. B) Point A has the lesser
More informationSTRENGTH of MATERIALS. P.A.Hilton Ltd. Two Year Warranty UNIVERSAL MATERIAL TESTER HARDNESS TESTERS DEFLECTION/FATIGUE IMPACT TESTERS POLARISCOPE
P.A.Hilton Ltd STRENGTH of MATERIALS P.A.Hilton Ltd is a market leader in the manufacture and provision of teaching equipment for Universities and Technical Colleges worldwide for both degree and vocational
More informationPHYSICS 111 HOMEWORK SOLUTION #9. April 5, 2013
PHYSICS 111 HOMEWORK SOLUTION #9 April 5, 2013 0.1 A potter s wheel moves uniformly from rest to an angular speed of 0.16 rev/s in 33 s. Find its angular acceleration in radians per second per second.
More informationCHAPTER 4 TENSILE TESTING
CHAPTER 4 TENSILE TESTING EXERCISE 28, Page 7 1. What is a tensile test? Make a sketch of a typical load/extension graph for a mild steel specimen to the point of fracture and mark on the sketch the following:
More informationTensile Testing of Steel
C 265 Lab No. 2: Tensile Testing of Steel See web for typical report format including: TITL PAG, ABSTRACT, TABL OF CONTNTS, LIST OF TABL, LIST OF FIGURS 1.0  INTRODUCTION See General Lab Report Format
More informationUniaxial Tension and Compression Testing of Materials. Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng
Uniaxial Tension and Compression Testing of Materials Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng 3.032 Lab Report September 25, 2013 I. Introduction Understanding material mechanics
More informationMohr s Circle. Academic Resource Center
Mohr s Circle Academic Resource Center Introduction The transformation equations for plane stress can be represented in graphical form by a plot known as Mohr s Circle. This graphical representation is
More informationGriffith theory of brittle fracture:
Griffith theory of brittle fracture: Observed fracture strength is always lower than theoretical cohesive strength. Griffith explained that the discrepancy is due to the inherent defects in brittle materials
More informationSOLID MECHANICS TUTORIAL MECHANISMS KINEMATICS  VELOCITY AND ACCELERATION DIAGRAMS
SOLID MECHANICS TUTORIAL MECHANISMS KINEMATICS  VELOCITY AND ACCELERATION DIAGRAMS This work covers elements of the syllabus for the Engineering Council exams C105 Mechanical and Structural Engineering
More information